3 4456 0 3 5 2 8 2 2 5
ORNL/Rv€-11955 Dist. Category UC-501 (Chemistry) Chemical Technology Division
LITERATURE INFORMATION APPLICABLE TO THE REACTION OF URANIUM OXIDES WITH CZHLORINEi TO PREPARE URANIUM TETRACIHLORIDE
Paul A. Haas
Date Published: February 1992
Prepared by the OAK RIDGE NATIONAL LABORATORY
Oak Ridge, Tennessee 37831 managed by MARTIN MARIETTA ENERGY SYSTEMS, INC. for the U. S. DEPARTMENT OF ENERGY
2.1 THERMOCmMICALDATA 2.2 PHASEDIAGRAMS
3 3 5
2.3 EXPERIMENTAL, RESULTS FOR CHLORINATION OF URANIUM OXIDES .................................................... 14 3.
DISCUSSIONS AND CONCLUSIONS .................................
........................ 17 SELECTION OF CHLORINATION CONDITlONS ..................22 SALT PROPERTIES AND CONTROL CONSIDERATIONS ...........24
3.1 THERMOCHEMICAL CONSIDERATIONS 3.2 3.3
3.4 PREPARATION OF TiCI.. ZrC1.. SiC1.. and ThCl. FROM OXIDES ....................................................
27 -28 -29
LIST OF TABLES
1 Physical properties of U-0-C1 compounds
2 Thermochemical data
3 Vapor pressure equations 4
Heats of formation for U-0-CI compounds at 298 K
5 Free energies of formation for U-0-CI compounds at 900 K (627°C)
LIST OF FIGURES
Vapor pressures of uranium chlorides
2 Phase diagram for UCl..UO.
3 Phase diagrams for the compounds of uranium and chlorine
4 Liquidus temperatures ("C) for UCI..MgCI..
5 Diagram €or log P,
vs log P.
Conversion reactions for U-0-C1 compounds and free energies
Solubility of UO. in UCI. and UF.
IJTERATURE INFORMATION APPIKABLE To THE REACI'ION OF URANIUMOXID= WITTI CHLORINE To PREPARE URANIUM TEI1RAcM;oRIDE Paul A. Haas
The reactions of uranium oxides and chlorine to prepare anhydrous uranium tetrachloride (UC14) are important to more economical preparation of uranium metal. The most practical reactions require carbon or carbon monoxide (CO) to give CO or carbon dioxide (Cod as waste gases. The chemistry of U-0-Cl compounds is very complex with valances of 3,4, 5, and 6 and with stable oxychlorides. Literature was reviewed to collect thermochemical data, phase equilibrium information, and results of experimental studies. Calculations using thermodynamic data can identify the probable reactions, but the results are uncertain. All the U-0-C1 compounds have large free energies of formation and the calculations give uncertain small differences of large numbers. The phase diagram for UCl,UO, shows a reaction to form uranium oqchloride (UOCI,) that has a goad solubility in molten UCl,. This appears more favorable to good rates of reaction than reaction of solids and gases. There is limited information on U-0-Cl salt properties. Information on the preparation of titanium, zirconium, silicon, and thorium tetrachlorides (TiCl,, ZrCl,, SiCI,, ThCl,) by reaction of oxides with chlorine (Cl,)and carbon has application to the preparation of UCI,.
1. INTRODUcxi[ON An anhydrous UCI, salt has the properties to be an important intermediate
chemical for processing and applications of uranium compounds. This was recognized during the World War I1 program to prepare nuclear weapons; preparation of UCI, was
studied at that time. These studies showed that uranium tetrafluoride (UF,) was much easier to prepare and handle than UCl,. Also,the uranium fluorides were better than
chlorides for gaseous diffusion separation of isotopes and for batch, bomb reductions to uranium metal. Therefore, most of the uranium that has been mined, concentrated, and purified to give uranium ore concentrates (uranium oxides) has been converted to UF,.
2 The use of uranium chlorides in place of uranium fluorides would have important economic advantages. The hydrogen fluoride (HF) and fluorine (I?,)
required to prepare
the uranium fluorides are expensive chemicals. Processes that use fluorine compounds end up with toxic and troublesome wastes, such as magnesium and calcium fluoride (MgF2 and
Cap2) and isotopically depleted uranium hexafluoride (UF,). If uranium chlorides were used, the recycle or reuse of the chlorides is more practical. The proposed installation of a new industry for enrichment of uranium isotopes could benefit from the economic advantages of using uranium chlorides. The feed to an Atomic Vapor Laser Isotope Separation (AVLIS) process will be uranium metal.' The
principal production of uranium metal for nuclear fuel cycles has previously been by batch
metallothermic reductions of UF, using magnesium or calcium metal. For a large enrichment plant ( > lo4 ton Uiyear), the costs of the HF feed, the calcium (Ca) or magnesium (Mg) feed, and the disposal of MgF, or CaF, waste are major parts of thc total uranium enrichment costs. Some alternate processes for preparation of uranium metal from UCl, allow recycle of Cl, from electrolytic cells. The application of these processes requires the reaction of uranium oxides with CI, to prepare UCI,.
The purpose and scope of this review is to collect, organize, and discuss the litera-
ture information useful to the reactions of uranium oxides and chlorine to prepare anhydrous UCl,. The review is selective in that only one set of consistent and useful rcsults i s presented without reference to less useful or inconsistent information. An excellent comprehensive and critical review of the chemistry of uranium was prepared as an account of work and information from the U. S. Manhattan Project., Such a review for the preparation of UCI, will not be repeated here. Well-organized and more complete presentations of thermochemical data for uranium compounds were published by Rand and Kubaschewski in 1963,3Fuger et a1 in 1983,4and Barin in 1989.5 An assessment of thermochemical data â‚Źor the system uranium-oxygen-chlorine by Cordfunke and Kubaschewski6illustrates the scatter of individual values, the limits of accuracies, and the dependence on estimated values. Selected values will be listed and discussed in the following sections without detailed rcference to these limitations.
The processes of interest for the preparation of the anhydrous UCI, are to react the uranium oxide feeds with chlorine (an oxidizing agent) and carbon or carbon monoxide (reducing agents). Oxidation and reduction reactions will take place and all possible uranium oxides, uranium chlorides, and uranium oxychlorides must be considered. Physical properties for these compounds are tabulated (Table 1). A consistent set of thermodynam-
ic data for these uranium compounds is needed to allow calculations to identi6 the probable reactions. The data for C, GO, and C 0 2 as reactants or products and for H,O and HCl as impurities are included for convenience. Phase diagrams are important as they present useful equilibrium results. Finally, results are reviewed for the reported experimental studies of the reactions of uranium oxides, chlorine, and a reducing agent. The principal component of a molten salt for a chlorination will probably be UCI,. Other physical information reported for UCI, include^:^ Heat of fusion at 863 K 44.8 kJ/mol Free energy of vaporization at 863 K 218 kJ/mol Entropy of vaporization at 1062 K: 133 J/mol K Densities of molten UCl, are: Temperature
650 700 750
3.55 3.45 3.36
The properties, preparation, and chemistry of the uranium chlorides and oxychlorides are comprehensively reviewed by Brown!
21 T " E M I c A L D A T A The application for the thermodynamic data is to make calculations at the chlorination reactor conditions. The most useful values are the free energies of formation at 700
to 1100 K A temperature of 700 K (427째C) is about the lowest temperature of interest for both practical rates of reaction and the use of molten chloride salts. The 1100 K
Table 1. Physical properties of U-0-CI compounds
Density at 298 K, (g/cm3>
Melting point (K)
Boiling point (K)
Color at 298 K
Olive-green Dark red
Dark grcen Green
Brown-black Black decom.
Black or dark green
"de~om.= decomposes without phase change,
5 (823Â°C) is above the boiling point of UCl, and is near the highest practical temperature. The enthalpies and entropies of formation at reference conditions are available for nearly all the uranium chlorides and oxychlorides, but the high-temperature data is much less complete. The enthalpies and free energies in recent (since 1975) assessments and collections of data are mostly 20 to 30 kJ/mol smaller (less negative) than those listed before 1970. It is probably inconsistent and misleading to use early and recent data together in one calculation.
A recommended set of data for calculations is tabulated (Table 2). This data is
from the more recent publication^./^^^â€˜^^ Data published for uranium chlorides and
oxychlorides before 1975 is not consistent with this more recent data. The significance of and conclusions from the thermochemical data are discussed in Sect. 3.1. Krahe listed vapor pressure equations as shown in Table 3.l' Calculated values
from these equations are shown in Fig. 1. The decomposition of UC1, (or UCI,) into Cl,
and UCl, must be considered; the UCl, or UCl, are stable only when excess Cl, is present.
2 2 PHASEDIAGRAMS
Phase diagrams present equilibrium information in several different ways. With only two components, a composition versus temperature type of phase diagram can show a complete representation of the solid, liquid, and gaseous phases present. The diagram for U02-UCl, gives information important to understanding the chlorination behavior. Most
of the other two-component phase diagrams for uranium oxides, oxychlorides, and chlorides are not available in published literature. For three components, a triangular diagram can
show one variable (usually the liquidus temperature) vs all compositions. A third type of phase diagram can be calculated from the thermodynamic data. The calculations give the equilibrium concentration or solid phases present vs two of the concentrations as
Table 2. Thermochemical data
at 298 K
S at 298 K (J/mol.K)
Free energy of formation (-A@') (kJ/mol) 700 K
187.03 198.08 241.83 208.81 188.83 "(E) indicates estimated values. %e term "na" indicates that values are not available in any of the known references.
ORNL DWG 9 l A - 1 1
400 200 100
20 10 8 6 4
TEMPERATURE ('6) Fig. 1. Vapor pressures of uranium chlorides.
8 Table 3. Vapor pressure equations'
298 - 1110
1110 - 1950
298 - 863
863 - 1062
298 - 600
298 - 453
The phase relationships between tetravalent uranium oxide and chloride are shown in Fig. 2.12 The phase diagram shows that there are three stable compounds over the entire range of composition---UC1,, UOCI,, and UO,. There is a eutectic reaction between
UCl, and the intermediate compound, UOCi,. The melting point of pure UCl, i s 590째C.
A minimum melting point of 545째C occurs at the eutectic Composition of UCI, % UO,.
A maximum solubility of about 13 mol % UO, in molten UC1, is reported at
810째C. At temperatures from 810 to 855"C, UCI, vapor is in equilibrium with solid
UOCl, UOCI, decomposes at 855째C. ,4t higher temperatures, vapor and solid UO, are in equilibrium. This phase diagram suggests practical limitations on the useful chlorination conditions and will be discussed further in this respect (Sect, 3.2).
A phase diagram with the Cl/U atom ratio as the concentration variable shows the melting points of the uranium chlorides and their eutectics (Fig. 3)." This diagram is a series of binary diagrams for U-UCI,-UCI,-UCI,-UCl, as no more than two of these compounds can be present in equilibrium.
Fig. 2. Phase diagram for UCI,-U0,'2
11 For reasons discussed in Sect. 3.2, a ternary mixture of UCl,-MgCi,-NaCl might be the preferred melt for reaction of UO,, C1, and C. While this ternary diagram has not been determined, the three binary diagrams (UCI,-MgCI2, UC1,-NaC1, MgC1,-NaCl) have been ~ub1ished.l~These binary diagrams give the liquidus temperatures for the three sides
of a ternary MgCI,-NaCl-UCl, phase diagram. The three binary diagrams are simple, and simple liquidus curves fur the ternary are very probable. Estimated curves were drawn (Fig. 4) with shapes similar to those for other published ternary diagrams. These curves are derived from the binary data and should be considered interpolations between them instead of extrapolations. An important use of thermochemical data is to calculate the equilibrium composi-
tions at specified temperatures. Uranium has five major valences (0, 3, 4, 5, 6) and also has some stable compounds of apparent intermediate valances (4.5, 5.33, 5.5). Only two of the major valences can be in equilibrium at a specified condition. Uranium and chlorine give a series of compounds (U, UCl,, UCl,, UCI,, UCI,). Each composition from Cl/U=O to C1/U=6 will have an equilibrium overpressure of Cl, gas. These equilibrium concentrations can be calculated from thermodynamic data. They can be conveniently represented by equations with temperature as a variable and do not require phase diagrams. The melting points and eutectics were shown in Fig. 3. Thermochemical data can also be used to calculate equilibrium compositions for the U-0-Cl system. Because of the multiple valances of uranium and the formation of oxychlorides, over twenty U-0-Cl compounds are possible. At least seventeen of these compounds have been reported experimentally.6 The results can be presented as diagrams showing the composition of the solid phase with a specified temperature as a constant and
two gas activities (C1, and 0, or CO) as the variables. A result of interest for the chlorination of UO, to UCI, is reported by Krahe (Fig. 5)"
Chlorine pressures near 1 atm
give a melt that consists of UCI, and UCI,. UCI, is the stable composition for a wide range of both C1, and CO (or 0,) concentrations. Krahe's result looks very good with respect to utilization of Cl, and the formation of UCl, as the product. Cordfunke discusses the U-0-Cl phase calculations and the limitations from the precision of the data.6 He
shows that small differences in the data can cause phases to appear or disappear from the calculated results. He estimates a need for 0.25% precision for enthalpies and 1%for entropies. The data for uranium oxychlorides is probably not this good. The poor
ORNL DWG 91A-634
a 2 w !-
ATOM RATIO OF CI/U
Fig. 3. Phase diagrams for the compounds of uranium and ~ h l o r i n e . ~
ORNL DWG 91A-630
DATA: BINARY-PHASE DIAGRAMS FOR UC14 -NaCI, UCl4-MgC12, AND MgC12-NaCi.13 ALL ISOTHERMS BY INTERPOLATION.
N a CI (800' C>
(71 4 O C )
Fig. 4. Liquidus temperatures ("C) for UCl,-MgCI,-NaCl.
O R N L DWG 91A-633
Fig. 5. Diagram for log P,
vs log PCl2at 400째C.11
information on the composition or chemical purity of the samples that were used is an important source of error. Cordfunke gives three phase diagrams for 0, and Cl, pressures as the concentration variables to illustrate the effects of small differences in data.6 Krake gives over twenty calculated results with gas concentrations, temperature, and the activity of carbon or CO as variables."
A search of technical literature did not reveal any significant reports for the preparation of pure UCl, from reaction of uranium oxides with C1, and C or CQ. There is extensive literature on the production of UCl, by reaction of carbon tetrachloride (GCl,) with uranium oxides.z14 One such process was used at Oak Ridge for producing calutron feed for isotope separations. The CCl, cannot bc produced by a simple reaction of C with Cl,, Therefore, the reactions of CCl, with uranium oxides do not provide efficient overall reactions of CI, to prepare UCl,. There are many literature descriptions concerning the reactions of chlorine with uranium oxides. Some of these were intended to produce uranium chlorides with some results for carbon as a reactant and CO, or CO as products. Experiments using chlorine gas feed to graphite distributors immersed in molten salts showed good rates of reaction of
CR,. These graphite distributors providc a carbon source of relatively low-surface area and
reactivity, and the rates of formation of CQ and CO, are much better than might be expected. Canning demonstrated nearly complete utilization of C1, for up to 90%
chlorination of uranium oxides in NaCI-MgCl, at 700 and 800째C.'5 Analyses indicate 80 to
85% UCl, and 15 to 20% UCl, at the end of chlorination. Gibson claims a similar result with all thc uranium soluble in the NaC1-KCI melt at the end of chlorination.'6 Gens studied the volatilization of uranium chlorides from nuclear fuels and appeared to find the formation of some non-volatile U0,Cl,.'7
Lyon reported rapid reactions of uranium oxides
in molten NaCI-KCl at 850째C with CI, to give U02C12.18 The reactions of uranium oxides with CCI, have been more carefully studied than the reaction with C1, and C or CO. Sincc the free energy of formation of CCl, is positive above 415"C, the use of CCl, above this temperature is somewhat thermodynamically
15 equivalent to use of C and Cl, Budayev provides good thermodynamic analyses and experimental results of reactions with CCl,.14 Reaction products at 200 and 300°C were UO, and UCI,, Reaction products at 400 to 700°C included UO, UCl,, UOCI,, UOCI,
The experimental results showed stepwise reaction with many intermediate products, including CO, COCla Cl,,and all the uranium oxychlorides.
Gens reported that the U,08 treated with CCI,-Cl, is first converted to UO,CI, and is then further reacted to give UCI,, UCl,, and UC&.19 Jangg found high conversions to volatile UCl, and UCl, at 700 to 900°C using CCI, while C1, gave mostly U02Cl,.20
Katz and Kabonowitch published an excellent review of the literature on the
chemistry of uranium up through 1946.2 The overall results for preparation of uranium chlorides indicate the following conclusions: 1. There were no complete and practical conversions of UO, to pure UCl, by reactions with chlorine and C or CO. 2. UO, was clearly the preferred uranium oxide feed. Uranyl compounds were much less reactive. Higher oxides, such as U308 and UO,, gave larger amounts of UCl, as compared to the UCl, yield from UO, at similar conditions.
3. The conversion of UO, to UOCI, appears to liberate more energy than the conversion of UOCl, to UCI,, Therefore, an incomplete conversion is likely to leave large amounts of UOCl, instead of unreacted UO, and UCl,, 4. The first reported preparation of UCI, was by the reaction of a U0,C mixture with Cl, gas. The major disadvantages were the major yield of UCI,, the high reaction tempera-
ture, and the phosgene in the waste gas.
5. The reaction of UO, with CCI, proceeds at lower temperature and gives less UC15 and phosgene than UO, with C and Cl, Common conditions were 350 to 450°C in CCI, vapor or 150 to 250°C in liquid CCl, under pressure. 6. Phosgene (COClJ was an effective reagent at temperatures of 450°C or higher.
7. The higher chlorides (UCl,, UCb) are formed when the higher oxides (U30,, UO,) are converted to chlorides and are also formed by reaction of UCl, with Cl,
3. DISCUSSIONS AND CONCLUSIONS
The application of literature information to plan a development program for UCl, preparation is given here. The use of thermodynamic data is the logical first step, but has important limitations. The experimental results reported in the literature show reactions of chlorine and uranium oxides with little information on what reactions are occurring. The chemistry and preparation of TiCl,, ZrCl,, ThCl,, and SiCl, have important similarities to those of UCL,. Therefore, references for preparation of these compounds are reviewed as
sources of information applicable to UCl,.
Uranium dioxide is one of the most stable metal oxides and has a larger free energy of formation than UCI,. This means that many of the reactions that might convert UO, to UCI, are thermodynamically unfavorable. The displacement of the oxygen in UO, by reaction with Cl, is not practical. While the rate of reaction of UCl, with air is low at
room temperature, the thermodynamic equilibrium is a high ratio of C12/0, in the gas. At
225째C or higher, UCl, reacts with air to release C1, The practical conversion of UO, to UCl, by a chemical reaction requires a reducing agent which yields an oxide product that is more stable than the chloride (k.,it does not react with UCl,). Carbon and carbon monoxide meet this criteria. Both have large free energies of formation while CCI, has a zero value at about 415째C and decomposes
thermally at higher temperatures. Hydrogen oxide and hydrogen chloride are about equally
stable, and the oxide (water) reacts with uranium chlorides to form HCl and UOCl, or UO,
The equilibrium pressure of H20 over UO, in HC1 gas is very small, and conversion
to UCI, by countercurrent treatment of UO, with HCI (as used to prepare UF, using HF)
is completely impractical. For the same reasons, UQ, prepared in aqueous solutions cannot be dehydrated to anhydrous UCl,. Thermal or other treatments give removal of HCI leaving UO, or UOCI, as the product. Thermodynamic calculations are a logical first step to identifying the probable chemical reactions for conversion of UO, to UCl,. The use of thermochemical data does not identify the probable reactions with any certainty or degree of confidence. There are
several major causes of uncertainty. Uranium chemistry is complex with stable valences of 3, 4, 5, and 6, and with stable o x ~ r c h l o ~ dU02C1, ~. and UOCI, are well known compounds
and others are possible. All of the possible products must be considered. The uranium chlorides are more volatile with increasing valence, but UC1, and UCl, are less stable with increasing temperature and decreasing C1, partial pressure. All of the uranium compounds have large heats OE formation, and calculating the free energy of these reactions usually results in a small difference from two large numbers. Small percentage uncertainties for the large numbers give large uncertainties for the differences. The relationships between the U-0-Cl compounds can be illustrated by a matrix listing. Data are available for heats and entropies of formation at 298 K for nearly all of these compounds (Tables 2 and 4). The free energies of formation at 900 K would allow more realistic and useful calculations. However, bccause thc free energy of formation data at high temperatures is much less complete, this matrix listing contains less certain or estimated values (Table 5).
Table 4. Heats of formation for U-0-Cl compounds at 298 K
Valence 0 3
5.33 or 5.5 6
U" UCI, 862.1 UCI, 1018.8
U UOCl 947.3 UOCl, 1069.4
(W2CI5 1098.7 UOC1, 1140.1
- (Heats of formation), H/mol U
19 Table 5. Free energies of formation for U-0-CI compounds at 900 K (627째C)
- (Free enerw of formation). kJ/mol U One 0
5.33 or 5.5
UOCI, 900 (Est.)
(UO),CI, 880 (Est.) UCI, 763
U0,Cl 960 (Est.) (UOd2C13 990 (Est.)
The complexity of the uranium conversion chemistry is partly shown by a diagram
giving the free energies of the simple oxidation and reduction reactions (Fig. 6). This diagram was simplified by omitting the compounds of U(4.5) and U(5.5) valences. It also does not show the reactions of two U-0-C1 compounds to give a third U-0-Cl compound. The reductions are shown for %C to %CO,. Similar conclusions would apply for C to CO
or CO to C02 as the three free energies are 197.9, 191.4, and 204.3 kJ at 900 K.. The three free energies are equal at 973 K (700"C), and the probable products from carbon are
CO, below 700 K and CO at higher temperatures. Some general conclusions from examinations of Tables 4 and 5 and Fig. 6 are: At a given valence state, the uranium oxychlorides are more stable than the chlorides. At a given valence state, the uranium oxides are more stable than the chlorides.
ORNL DWG 9 1 A - 6 3 2 O/U,
I 1 I
CHLORINATIONS; FREE ENERGY IN kJ/ATOM
------eOXIDATIONS; FREE ENERGY IN kJ/(O -DISPLACEMENTS;
FREE ENERGY IN kJ/[O
REDUCTIONS; FREE ENERGY IN kJ/(C-CO)
Fig. 4. Conversion reactions for U-O-Cl compounds and free energies at
All additions of chlorine to oxides or oxychlorides of lower valence [less than U(VI)] are favorable to yield oxychlorides of higher valence.
The oxychlorides can be formed by both direct reaction of chlorine and by reaction of a uranium chloride with an oxide or oxychloride. Since oxychlorides are the intermediate compounds for conversion of UO, to UCl,,
their stability can be of critical importance to complete conversions. A conversion may appear favorable overall, but one of the steps for the intermediate may be much less favorable. For example, consider the following overall reaction:
+ 2 c + 2c1,
At 900 K, AG = -214.3 kT, but individual steps show:
UO2 C12 + UO,Cl,, AG = -29.2; U02C1, + C UOC12 .f CO, AG = -94.4; UOCI, f C1, UOCl,, AG = -37.0; and UOCI, + C UCI, + CO,AG = -54.
These numbers indicate that the reactions should take place, but older data indicate they could stop at UO,Cl, or UOCI,. If using CO to give CO, as the product is considered, then the two reduction reactions change to: U02C123- CO -, UOCI, + C O , AG = -107.3 and UOCl, + CO UCl, -tCO,,AG = -66.6. -+
The uncertainties for ArGovalues of U02C1, and UOCl, may be larger than the above AG values, so it is difficult to be certain that the reactions are thermodynamically favorable. The more favorable calculation for CO as compared to C may also be misleading. The C would be present as a solid with a thermodynamic activity of 1, while GO would be mixed with other gases and would have a lower activity for 1 atm total pressure. Many of the reactions to change between the U-0-C1 compounds are shown in Fig. 6. Large values for the negatives of the free energies of reaction (kJ/equiv at 900 K) show reactions that are thermodynamically favored. Positive values in Fig. 6 indicate that the
reactions are not t ~ e r ~ ~ o d ~ a ~favorable. i c a ~ l yThe data for the mychlorides are uncertain, and values ranging from -20 to +20 k;T do not justify predictions. Thc formation of UC1, and UCl, appears to require cxcesses of C1, and will not be complete. Otherwise, all additions of C1, arc favorable, and oxychlorides should add chlorine to givc U02CI, or UOCI,. The reductions of UO, or V,O, to UO, are highly favorablc. The reduction of
UOCI, to give UC1, is unfavorable. Some of the other reactions give free energies of reaction that are too near zero to justify predictions. A practical preparation of UCI, probably requires that the chlorinations to U(VI) and the reductions of UO,CI, and UOCI, be possible since the intermediates would otherwise accumulate as stable products. The equilibrium mixture among the uranium compounds for normal operation of a chlorination reactor will always be UCI, and uranium oxychlorides containing one oxygen. The feed of UO, will bc limited to prevent excessive solids; therefore, O/U ratios will be much less than one. Because of the lower stability of the chlorides as compared to the oxychlorides, any uranium compounds containing two oxygens will react with a uranium chloride to form two oxychlorides with one oxygen in each. Any U(V1) or U(V) will be much more stable as oxychlorides than as UC1, or UC1,. Therefore, the amounts of UCI, and UCl, will be small unless the moles of U(VI) and U(V) exceed the moles of oxychlorides. Some of thc reactions and their free energies at 900 M are:
UCl, +U0, + 2UOC1,, A G = -32.9 kJ; UC15 + UO$.I+2UOCl,,AG -53.9 kJ; UCR, lJO,Cl2 4 2UQCI4, A G == -80 kJ, UCl4 + UO,C%,--P 2UOCI3, A G -54.3kJ; UCI, + UO, -+ UO,Cl, -b UCl,, A G = -31.5 kT; and UCI, + WOC12 + UOC1, + IJCl,, A G -39.3 kJ.
The first five reactions indicate that the uranium chlorides will react to give oxychlorides. 'Ibc first four show that an oxychloride containing two oxygens will react with uranium
chlorides to givc two oxychlorides. Tke last two show that UCI, kill react with a U(IV) oxychloride to give UCl, and an U(V1) oxychloride.
One feed material must be the uranium oxides from ore refineries. Recycling considerations to eliminate large amounts of waste require the use of C1, gas from electrolytic cells.
23 Thermochemical data show larger free energies of formation for uranium oxides than for chlorides of the same valence. Therefore, the overall reaction must include a reducing agent that has a much more stable oxide than chloride. Carbon or carbon monoxide are the most practical reducing agents that meet this requirement. Hydrogen (as H2or hydrocarbons) does not meet this requirement since H,O will react with uranium chlorides to form HCl. Sulfur and phosphorus (and some of their compounds) can meet this thermochemical requirement, but they are expensive feeds and give troublesome waste oxides in comparison to carbon. The overall reaction from the above considerations shows one or two solids (uranium
oxides, C) and gaseous feed (C12 perhaps CO) and a gaseous product (CO, or CO). Even with stepwise reactions, the reactions between two phases with one of them a solid tend to be slow or incomplete. The phase diagram for UO, and UC14 (Fig. 2) shows several
indications toward practical conditions for conversion of UO, into UCI,. The use of a liquid melt with reaction of UO, and UCI, to give UOCI, in solution appears favorable to high rates of reaction. Then the C1, and carbon can react with the UOCI, or other oxychlorides in solution. The Cl, can also react with UCl, to give UC1, or UCl, as soluble chlorinating agents in the melt. Both the temperature and the fraction of UO, in the charge must be limited to maintain the desirable liquid melt condition. All of the UO, reacts with UCl, to form UOC1, and any UOCI, above the solubility is present as solids. An equimolar mixture of UO, and UCI, gives all UOC1, solids without any melt. Since C will also be a solid, the preferred concentration to ensure a fluid melt will be less UO, than the solubility limit (from 6.9 mol % at 545째C to about 13 mol % at SIO째C). The preferred temperatures will
be intermediate between the melting point and boiling point of UCI, (590 to 792째C). The vapor pressure of UCI, is also an important consideration.
The addition of a diluent salt to the melt would relax some of the composition and
temperature limits indicated by the UC14-UO2 phase diagram. The diluent salt should be unreactive with the carbon, C12, UO,, and UCI,, should have a low volatility at 600 to W " C , and should melt below 600째C. An equimolar mixture of MgC1,NaCl meets these requirements better than any single salt. Mixtures of MgCl,-NaCl are commonly used for electrolytic production of Mg and C12 and have good properties. There are no published phase diagrams for UC1,-U02-MgC1,-NaC1 or for any ternary mixtures of these components. However, reasonable liquidus temperatures and UO,
solubilities can be estimated from four binary phase diagrams. Binary diagrams for MgCI,NaCl, MgCI,-U@l,, and NaC1-UC1,'3 can be used to give liquidus temperatures for the three sides of a ternary MgCI,-NaCl-UCl, phase diagram. The three known binary diagrams are all simple and simple liquidus curves for thc ternary are very probable. Estimated curves were drawn (Fig. 4) with shapes similar to those for other published ternary diagrams. The UCI,-UO, binary phase diagram gives the data needed for a UO, solubility versus temperature in units of moles U02/ITC14 (Fig. 7). Experimental data €or fluoride salt mixtures show that the UO, solubilities are proportional to the UF, concentration; that is, rnolcs UO,/moies UF, is dependent on the temperature and the other salt compositions but independent of the UF, concentration. Figure 7 shows the data €or the solubility of UO, in IJF, also. The data €or UC1, and UF, could be represented by a single curve. Considering the MgC1,-NaCl-UCl, ternary together with the UO,-UCl, binary, it is likely that replacement of part of the UCl, by UO, up to the solubility limits shown by Fig. 7 would have only small effects on the liquidus temperatures of Fig. 4. As an example of the results of these assumptions, a charge of 20 mol % MgC1,-20 mol % NaC1-6(0 mol 96 (UCI,+UO,) would be expccted to be all liquid above 500°C with UO, solubilities from 4 mol % at 500°C to 8 mol % at 800°C 3.3 SALT PRQPERTIFS AND PRO
The practical chlorination of uranium ore concentrates to UCI, on a large scale would require continuous processes with controlled inventories of the process materials. The literature data indicate that a molten salt reaction with feeds of UO,, Cl,, and C or CO might be most practical. The UCI, product must have low concentrations of unreacted carbon or oxygen. Large amounts of unreacted chlorine in the product gas are also very undesirable. Countercurrent flaws with high conversion to UCI, in a melt (low oxychlorides, lJC15 and UCl,) would be extremely difficult to accomplish. A more practical concept is to remove UC1, as a vapor from a melt with compositions favorable to high utilizations of the C1, feed. The chlorination reactor will have three reactant feed streams and two products leaving the reactor. The most likely overall reaction will be one of: UO, + c 4- 2c1,4 UCl, IJO, f 2CO + 2C1, * UC1,
+ CO, f
ORNL DWG 91A-631 0.40
AT >,855' C
5 .**. F R O M UCI,-UO, DtS SOLVED UO,
PHASE DIAGRAM?^ IS UOCI,
FOR UF4 (GREENFIELD AND HYDE IN AERE-R 6463)
Fig. 7. Solubility of UO, in UC1, and UF,.
Reactions with either CO or carbon and with other uranium oxides as feed will also have five primary flows of fceds and products. Small amounts of unreacted CI, or of CO in addition to CO, and large amounts of a nonreactive diluent gas (N, or CO,) do not change the need to control five process inventories or process flows. All gases including thc gaseous products, unreacted C1, or CO, and nonreactive diluent gas leave by displacement without need for a control measurement. This leaves four other flows requiring control.
One flow can be set to cstablish the system capacity. This is most logically the. C1, feed rate. Since there is little or no chlorine inventory in the mclt, a change in the chlorine feed rate can give an immediate change in the rate of C1, reactions. It would normally be desirable to have a good inventory of UO,, C, or CO and the molten chloride salt to allow high utilizations of C1,. Depleting one of these charge cornponcnts to provide control of the rcaction rate contributes to high, undcsirable losses of urireacted Cl,. The condensed phase in the chlorination reactor is likely to contain more UCl, than
any other component. Therefore, it is logical to measure the condensed phase level or e and use this measurement to control the UCI, exit rate. The gas leaving the
charge should be at a vapor pressure equilibrium; that is, saturated with UCI, vapor. The UCl, vapor rate could be changed by changing the charge temperature (to increase the vapor pressure of UCI,) or by changing a diluent gas rate. Liquid or solid UCl, could be recycled to the charge to control the net outflow of UCl,. Use of nonvolatile diluent salts such as CaCl,, MgCI,, or NaCl would reduce the vapor pressure of UCI, by reducing the UCL, concentration. The diluent salts could provide some automatic changes in the rate of UCl, vapor. When the UC1, is depleted, the lower concentration of UCl, would result in a
lower rate of vaporization. Excess UCI, would result in a higher rate of UCl, vaporization.
For pure UCl,, concentration in the melt and the vapor pressure do not change as the amount in the charge varies. After the sates of gas exit flow, C1, feed, and UCl, vapor are determined as described, the feed rates of UO, and C or CO remain io be controlled. While the rate of C1, losscs to the exit gas can depend on the charge inventories, measurement of CI, losses is a
poor control criteria. A high utilization of C1, is desirable and conditions that allow
increases in C1, losses are undesirable. Also, increases in C1, losses could result from
deficiencies in either UO,, or C-CO and could also result from excessive UOCI, or C solids
with poor gas-charge contact. Since a high CI, loss might have several causes, it would not be a dependable control measurement for one feed. The UQ, and C feed rates should be
controlled on a long-term basis by some direct measurement on the reactor charge-either measurements of salt properties or analyses of samples for C and oxygen. A review of the limited literature on uranium salt properties did not indicate any promising possibilities for use of measurements of the salt properties at ciao to 800째C. Based on the lack of information for measurement and use of salt properties for control, the UQ, and C feed rates will probably be set to agree with the C1, feed rate with
periodic adjustments from analyses of charge samples. Good inventories of UO, and C
appear desirable both to ensure good utilization of c1, and to make control from periodic samples more practical.
3.4 PREPARATION OF TiCl,,zrci, Sa,,AND I%Cl, FROM OXIDES
The chemistry and preparation of these metal chlorides have important similarities to those of UCI,. For all of them, the tetrachlorides have been produced from oxides using
Cl, and carbon as follows: MQ, + C + 2C1,4 CO,, -tMCI,,,, or MO, f 2C 2C1, -+ 2CO,, + MCI,,.
The ThCI, preparations were small scale. The other three conversions have been produc-
tion processes and should provide practical information that applies to production of UC&.
For silicon, the free energy of reaction is positive, but the reactions can be completed by removal of the SiCI, gas. This conversion of TiO, to Tiel4is used on a large scale (106 tonslyear) to prepare titanium dioxide pigments. The TiCI, is a more volatile product (mp 248 K and bp 409 K) than UCl,, and can be handled as a liquid at room temperature. While the process concepts for preparation of TiC1, are old and well known, the detaiIs of plant design and operation are proprietary with little publication as technical literature. The descriptions published in the 1950s2' and 1980sn are very similar.
One description of a plant opcsatbn is as follows: A rnkture of 20 to 30 wt %
calcined coke and 70 to 88 wt % TiO, ore is fluidized at 900to 1080째C using GI, gas. The reactor is lined with SiO, brick and some oxygen feed may be used to preheat the reactor or replace heat losses (the chlorination reactions are exothermic). The exit gases contain thc TiCI, product as vapor, some exccss Cl, CO,,and GO (ratios near 2 moVmol), and
volatile chlorides of impurity metals such as Fe, Mn, Cr, and A. The chlorides are
separated using the differences in volatility and melting points to give a purified TiC1, liquid as the product. An alternate to thc fluidized bcd is to flow the chlorine up through a
fixed bed of Ti0,-carbon briquettcs. Electrical resistance heating may bc used to
generate supplementary heat in the fixed bed. The use of S O , brick linings without excessive attack is possible as a result of the low surface area of the brick as compared to the mixture of fine SiO, and carbon that is used for preparation of SiC1,. A similar chlorination of Zr02-C briquettes at 6o(3-8OooCwas develope tion of Z ~ C I , .Fixed ~ beds of a - c m diam were operated using z~O,-C briquettes to
produce 100 mol ZrCl&
The ZrC1, leaves the reactor as vapor and is collected as con-
densed solids. ThCl, has bcen prepared using by reacting crushed ThO,-C compacts with C1, in a KCI-NaCl melt at 900째C." Careful operation was required to give complete conversions to TkCI, without residues of ThOCl,. The containcrs wcre silica (quartz).
This review resulted from a devclopmcnt program for preparation of uranium metal
feed for the AVLIS (Atomic Vapor Laser Isotope Separation) program. Discussions with and suggestions from H. W. Hayden, J. C. Mailcn, and M. J. Stcphenson contributed to the evolution of the review. Some references were supplied by H. W. Hayden and W. D. Bond. h y oversights or errors in the selection of data and the discussion and conclusions
are the responsibility of the author. The information in this review was used to plan and correlate results for a laboratory study. The experimental results show high rates of chemical reaction, good utilizations of chlorine, and collection of condensed UCI, product?
1. Phillip G. Sewell and Norman Haberman, "AVLIS Program Powers Ahead in the United States," Nucl. Eng. Int., pp. 17-19 (October 1988).
2. Joseph J. Katz and Eugene Rabinowitch, The Chemktry of Uranium, Pari 1. The Element, Its Binaly and Related Compounds, McGraw Hill (1951). 3.
M. H. Rand and 0. Kubaschewski, The Thrmochemical Properties of Uranium Compounds, Interscience Publishers (1963).
J. Fuger et al., The Chemical Thermodynamics of Actinide Elements and CompoundsPart 8: The Actinide Halides, International Atomic Energy Agency, Vienna (1983).
5. Ihsan Barin, Thermochemical Data of Pure Substances, Cambridge, New York (1989). 6.
E. H. P. Cordfunke, "Basic Thermodynamic Data in Nuclear Technology: New Developments, Old Problems," J. of Nucl. Mater., 130, 82-93 (1985).
David Brown, ''Compounds of Uranium with Chlorine, Bromine, Iodine," Gmelin Handbuh der Anorganischn Chemie, Vol. C9 (1979).
E. H. P. Cordfunke et al., Thermochemical Data for Reactor Materials an Fission products, Eur.-Contract no. ETSN-0005-NL (1988).
E. H. P. Cordfunke and 0. Kubaschewski, "The Thermochemical Properties of the System Uranium-Oxygen-Chlorine,"Themzochim. Acta, 74, 235-245 (1984).
10. M. W. Chase et al., JANAF Themzochernical Tables, Third Edition, h e r . Chern. Soc., Am. Inst. Physics, and National Bureau of Standards (1986). 11. Josef Krahe and Franz Muller, "Zur Thyermochernie der Stoffsysterne U, Th, Pa, C, O,, Cl,," Institute fw Chemisehe Techmlogie, Jul565-CT (December 1968). 12. Y. M. Sterlin and V.V. Artamonov, cited by E. M. Levin and H. F. McMurdie, Phase Diagrams for Ceramists: 1975 Supplement, The American Chemical Society, Columbus, OH, 1975, p. 396. 13. H. E McMurdie, Editor, Phase Diagrams for Ceramists, Vol I to VI& American Ceramic Society (1964 to 1989).
14. I. V. Budayev and A N. Volsky, "The Chlorination of Uraniun Dioxide and Plutonium Dioxide by Carbon Tetrachloride,"Roc. of Second United Nations International Con. on the Peaceful Uses ofAtomic Enew, p.2195, pp. 316-330, (1959). 15. R. G.Canning, 'The Production of Uranium Metal Powders by Electrolysis in Molten Chlorides,"Australian Atomic Energy Symposium-1958, pp. 115-122 (June 1958).
16. k R. Gibson et a!., "Processes for the Production of Uranium &de," U. S. Patent 3,117,386 (January 14, 19
17. T. A- Gens, Laboratory Development of Chloride Volatility Processes for the Recovery of Uranium Directly from Spent Rover Fuel orfiom its CombustionAsh, ORNL-3376 (June 1963). 18. W. L. Lyon and E. E. Voiland, The Reparation of Uranium Dioxide from a Molten Salt Solution of Uranyl Chloride, HW-62431 (October 1959).
19. T. A. Gens, Chloride Volalility ental Studies: The Reaction of U,O, with Carbon Tetrachloride and Mixtures of Carbsrz Tetrachloride and Chlorine?,ORNLA?d1258 (August 1965).
20. G. Jangg et al., "Chlorination of Uranium Oxides,"Atornprmis, 7, 332-336 (1961). 21. A. a>. Mcquillan and M. K. McQuillan, Titanium, Academic Press (1956). 22. Minoru Qgawa et al., "A Study of Titanium Resources and Its Chlorination Process," Titanium '88 Science and Technology, pp. 1936-1945, Kyoto, Japan (May 19-22, 1980). 23. S. M. Shelton et al,, "Zirconium Metal Production," Proc. of the Internalional Conj on the Peaceful Uses of Atomic Energy, 8, 505 (1956).
24. A. W. Gibson et al., "Thorium Metal Production by a Chlorination Process,"Proc. of Second United Nations Intematiomil Conf on the Peaceful Uses of Atomic Energy, 4, 237-242 (1959). 25. P. h P'laas et al., Reachn of Uranium Oxides with Chlorine and Carbon or Carbon Monoxide to Prepare Uranium Chlorides, ORNLflM-11792, Oak Ridge National Laboratory (November 1991).
Dist. Category UC-501 (Chemistry)
D. M. Andrew J. T.Bell W. Fulkerson R.K. Genung 5-9. P. A Haas 10. H. W. Hayden 11. W. H. Kermes 12. J. R. Hightower 13. K H. King-Jones 14. F. E. Kosinski 15. L. k Lundberg 1. 2. 3. 4.
16. 17. 18. 19. 20. 21.
22. 23. 24. 25. 26.
J. C.Mailen J. R. Merriman J. A. Pashley A. S. Quist M. H. Randolph K-25 Records Depart. Enrichment Technol. Cen. Research Library Document Ref. Section Lab Records, ORNL RC ORNL Patent Section
27-36. Ofice of Scientific and Technical Information, Department of Energy, P. 0. Box 2001, Oak Ridge, TN 37831
37. Office of Assistant Manager, Energy Research and Development, Oak Ridge Operations, P. 0. Box 2001, Oak Ridge, TN 37831 38. N. Habermann, U. S. Department of Energy, Washington, D.C. 20585 39. J. k Horton, Lawrence Livermore National Laboratory, P. 0. Box 808, Livermore, CA 94550 40-136. Given distribution as UC-501,Nuclear Energy (Chemistry)